damp.htmlhttp://www.kettering.edu/~drussell/Demos/SHO/ damp.html The black mass is undamped and the blue mass is damped (underdamped). After being released from rest the undamped (black) mass exhibits simple harmonic motion while the damped (blue) mass exhibits an oscillatory motion which decays with time.
Damping is the conversion of mechanical energy of a structure into thermal energy. The amount of energy dissipated is a measure of the structure’s damping level. Damping is very important with earthquakes since it dissipates the destructive energy of an earthquake which will help reduce the damage to the building.
D oo oo Hysteresis loop for a viscoelastic material D = energy dissipation per cycle Stress Strain
Superelastic behavior T > A f Hysteresis loop means energy dissipation, hence vibration damping Stress
The more is the hysteresis in the stress-strain curve, the greater is the energy dissipation, and hence the higher is the damping ability.
Consider the suspension of your automobile, supporting the body mass. You have four springs. You also have four friction elements, variously called dampers or dash pots or shock absorbers. Don’t try to drive without them! Here are some friction elements – dampers – that you can see.
Let’s diagram our hardware. We have a “sprung mass” M and a spring with stiffness K. We also have a friction or damping element C. C is not always visible, but is always present. No system exists without some damping
Damping is the decrease in amplitude with time due to the resistance of the medium to the vibration.amplitude mediumvibration Damping occurs progressively as energy is taken out of the system by another force such as friction. If the damping is enough that the system just fails to oscillate, then it is said to be critically damped. Damping more than this is referred to as over damping and less is similarly underdamped.oscillate
Critical damping The minimum damping that will prevent or stop oscillation in the shortest amount of time.damping
Underdamped Transient response
Q = amplification factor (ratio of the response amplitude at resonance ω 0 to the static response at ω = 0)
Half-power bandwidth method (3 dB method) Loss factor
Vibration damping Passive damping Active damping
Viscous material A material in which the strain develops over a period of time and the material does not go to its original shape after the stress is removed.
Viscoelastic material A material in which the total strain developed has elastic and viscous components. Part of the total strain recovers similar to elastic strain. Some part of the total strain recovers over a period of time. Examples: polymer melts.
The combined viscous and elastic behavior (viscoelasticity) can be examined by determining the effect that an oscillating force has on the movement of the material.
All the energy stored during loading is returned when the load is removed. Stress is proportional to strain. φ = 0°
The material does not return any of the energy stored during loading. All the energy is lost once the load is removed. Stress is proportional to the strain rate. φ = 90°
Some of the energy stored is recovered upon removal of the load; the remainder is dissipated in the form of heat. The angel φ (0 < φ < 90°) is a measure of the damping level.
Viscosity Measure of resistance to flow Defined as the ratio of shear stress to shear strain rate Unit: Poise or Pa.s 1 Pa.s = 10 P = 1000 cP
The viscosity (η) is the tendency of the fluid to resist flow and is defined by:
(c)2003 Brooks/Cole, a division of Thomson Learning, Inc. Thomson Learning ™ is a trademark used herein under license. Shear-stress strain- rate relationships for Newtonian and non-Newtonian materials
G* = G' + iG'' where G* is the complex shear modulus, G' is the in-phase storage modulus and G'' is the out-of-phase similarly-directed loss modulus; G* = √(G' 2 + G'' 2 ).
tan δ = G''/G' where tan δ (also called loss tangent) quantifies the balance between energy loss and storage. As tan 45° =1, a value for tan greater than unity indicates more "liquid" properties, whereas one lower than unity means more "solid" properties, regardless of the viscosity.
G* = G' + iG'' G is the storage modulus and G'' is the loss modulus; The frequency where these parameters cross over corresponds to a relaxation time ( ) specific for the material.
Application of a Tuned Vibration Absorber (TVA) is sometimes the best option for control of unwanted noise/vibration. This countermeasure is particularly appropriate when the noise/vibration issue occurs for a single frequency, or across a very narrow frequency range.
A variable damping system based on magnetorheological fluid sponges can help control the vibratory motion of a household washing machine during its spin cycle. Damping is switched on as the drum passes through resonance and off again at the highest speeds for optimum vibration isolation. The system permits the drum to rotate at speeds high enough to function as a centrifuge, but without the violent shaking familiar to every user.
Conventional springs and magnetorheological dampers work together to stabilize a home washing machine during the spin cycle.
A simple, inexpensive magnetorheological fluid sponge designed for incorporation into washing machines consists of a steel bobbin and coil surrounded by a layer of foam saturated with MR fluid. The elements constitute a piston on the end of the shaft that is free to move axially inside a steel housing that provides the magnetic flux return path. The damping force is proportional to the sponge's active area.
By activating the damper while the washing machine tub is passing through resonance, a degree of vibration control is achieved not possible with conventional springs alone. The damping mechanism is switched off at the greatest speeds, when the mechanical springs provide vibration isolation.
Constrained layer damping Embedding a viscoelastic layer in a structural material Shear deformation of viscoelastic layer provides energy dissipation.
Damping due to interfaces Slight slippage at interface during vibration providing a mechanism for damping
Damping due to defects Defects such as dislocations contribute to damping.
Use of interfaces for damping Discontinuous nanofiber between continuous conventional fiber layers for damping enhancement Tough competition with composites with viscoelastic interlayer for damping
Carbon nanofiber Fishbone morphology 0.16 micron diameter Discontinuous Intertwined Hollow channel along axis of nanofiber Grown catalytically from methane
Nanofiber as interlaminar filler Nanofiber enhances both transverse and longitudinal vibration damping ability (due to large area of the interface between nanofiber and matrix) Nanofiber increases the transverse storage modulus (due to presence of nanofibers that are oriented near the direction perpendicular to the fiber layers) Nanofiber decreases the longitudinal storage modulus slightly.
Table 1 Damping capacity (tan ) and storage modulus of cement-based materials at room temperature, as determined by flexural testing (three-point bending). Note that cement paste has no sand, whereas mortar has sand. _____tan ____ Storage modulus (GPa) 0.2 Hz1.0 Hz0.2 Hz1.0 HzRef. 1. Cement paste (plain)0.035< /23 2. Cement paste with untreated silica fume a Cement paste with treated b silica fume a Cement paste with untreated silica fume a and silane c 0.055/17.9/23 5. Cement paste with untreated carbon fibers d and untreated silica fume a Cement paste with untreated carbon fibers d and treated b silica fume a Cement paste with treated b carbon fibers d and untreated silica fume a Cement paste with treated b carbon fibers d and treated b silica fume a Cement paste with untreated carbon filaments d and treated b silica fume a a 15% by mass of cement b Treated by silane coating c 0.2% by mass of cement d 0.5 vol.% e 1.0 vol.% f 30% by mass of cement a. 15% by mass of cement, b. Treated by silane coating, c. 0.2% by mass of cement, d. 0.5 vol.%, e. 1.0 vol.%, f. 30% by mass of cement
Table 1 Damping capacity (tan ) and storage modulus of cement-based materials at room temperature, as determined by flexural testing (three-point bending). Note that cement paste has no sand, whereas mortar has sand. (Cont’d) _____tan ____ Storage modulus (GPa) 0.2 Hz1.0 Hz0.2 Hz1.0 HzRef. 10. Cement paste with treated b carbon filaments d and treated b silica fume a Cement paste with untreated steel fibers d and untreated silica fume a Cement paste with untreated steel fibers e and untreated silica fume a Cement paste with latex f // Mortar (plain)< Mortar with treated b silica fume a Mortar with untreated steel rebars Mortar with sand blasted steel rebars Mortar with untreated steel rebars and treated b silica fume a. 15% by mass of cement, b. Treated by silane coating, c. 0.2% by mass of cement, d. 0.5 vol.%, e. 1.0 vol.%, f. 30% by mass of cement
Table 1 Dynamic flexural behavior of materials at 0.2 Hz. Material tan Storage modulus (GPa)Loss modulus (GPa) Cement paste (plain) Mortar (plain)< < Mortar with silica fume (treated) (15% by wt. of cement) Aluminum, pure Al/AlN p (58 vol.%) Zn-Al Zn-Al/SiC w (27 vol.%) Carbon-fiber epoxy-matrix composite (without interlayer) Carbon fiber epoxy-matrix composite (with vibration damping interlayer) Neoprene rubber PTFE PMMA PA Acetal Epoxy